# chapter 5: diffusion in solids diffusion

Post on 02-Jan-2017

228 views

Embed Size (px)

TRANSCRIPT

1/28/2011

1

Chapter 5 - 1

ISSUES TO ADDRESS...

How does diffusion occur?

Why is it an important part of processing?

How can the rate of diffusion be predicted forsome simple cases?

How does diffusion depend on structureand temperature?

Chapter 5: Diffusion in Solids

Chapter 5 - 2

Diffusion

Diffusion - Mass transport by atomic motion

Mechanisms Gases & Liquids random (Brownian) motion Solids vacancy diffusion or interstitial diffusion

1/28/2011

2

Chapter 5 - 3

Interdiffusion: In an alloy, atoms tend to migratefrom regions of high conc. to regions of low conc.

Initially

Adapted from Figs. 5.1 and 5.2, Callister 7e.

Diffusion

After some timeCu Ni

Chapter 5 - 4

Self-diffusion: In an elemental solid, atomsalso migrate.

Label some atoms After some time

Diffusion

A

B

C

DA

B

C

D

Diffusion is just a stepwise migration of atoms from lattice site to lattice site.

There must be an empty adjacent site.The atom must have sufficient energy to break bonds with its neighbor atoms and them cause some lattice distortion during the displacement.

1/28/2011

3

Chapter 5 - 5

Diffusion Mechanisms

Vacancy Diffusion: atoms exchange with vacancies applies to substitutional impurities atoms rate depends on:

--number of vacancies--activation energy to exchange.

increasing elapsed time

Chapter 5 - 6

Simulation of interdiffusionacross an interface:

Rate of substitutionaldiffusion depends on:--vacancy concentration--frequency of jumping.

(Courtesy P.M. Anderson)

Diffusion Simulation

http://www.phys.au.dk/camp/m-t/

http://www.physics.leidenuniv.nl/sections/cm/ip/projects/dynamics/incopper/incopper.htm

1/28/2011

4

Chapter 5 - 7

Diffusion Mechanisms

Interstitial diffusion smaller atoms can diffuse between atoms.

More rapid than vacancy diffusionAdapted from Fig. 5.3 (b), Callister 7e.

Chapter 5 - 8

Adapted from chapter-opening photograph, Chapter 5, Callister 7e. (Courtesy ofSurface Division, Midland-Ross.)

Case Hardening:--Diffuse carbon atoms

into the host iron atomsat the surface.

--Example of interstitialdiffusion is a casehardened gear.

Result: The presence of C atoms makes iron (steel) harder.

Processing Using Diffusion

1/28/2011

5

Chapter 5 - 9

Doping silicon with phosphorus for n-type semiconductors: Process:

3. Result: Dopedsemiconductorregions.

silicon

Processing Using Diffusion

magnified image of a computer chip

0.5mm

light regions: Si atoms

light regions: Al atoms

2. Heat it.

1. Deposit P richlayers on surface.

silicon

Adapted from chapter-opening photograph, Chapter 18, Callister 7e.

Chapter 5 - 10

Diffusion How do we quantify the amount or rate of diffusion?

Measured empirically Make thin film (membrane) of known surface area Impose concentration gradient Measure how fast atoms or molecules diffuse through the

membrane

( )( ) smkg

orscm

moltimearea surface

diffusing mass) (or molesFlux 22=J

dtdM

Al

AtM

J ==M =

massdiffused

time

J slope

1/28/2011

6

Chapter 5 - 11

Steady-State Diffusion

dxdC

DJ =

Ficks first law of diffusionC1

C2

x

C1

C2

x1 x2

D diffusion coefficient

Rate of diffusion independent of timeFlux proportional to concentration gradient =

dxdC

12

12 linear ifxxCC

xC

dxdC

=

Driving Force---concentration gradient

Chapter 5 - 12

Steady-state diffusion

!"#

$%&'

("$&)("$&

#"*!

("$&("$&

"

Jx = D

dCdx

dCdx

left

=dCdx

right

+ ("& )("&

, -

1/28/2011

7

Chapter 5 - 13

Example: Chemical Protective Clothing (CPC)

Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn.

If butyl rubber gloves (0.04 cm thick) are used, what is the diffusive flux of methylene chloride through the glove?

Data: diffusion coefficient in butyl rubber:

D = 110x10-8 cm2/s surface concentrations:

C2 = 0.02 g/cm3C1 = 0.44 g/cm3

Chapter 5 - 14

scm

g 10 x 16.1

cm) 04.0()g/cm 44.0g/cm 02.0(

/s)cm 10 x 110( 2

5-33

28- ==J

Example (cont).

12

12- xxCC

DdxdC

DJ=

Dtb 6

2=

gloveC1

C2

skinpaintremover

x1 x2

Solution assuming linear conc. gradient

D = 110x10-8 cm2/s

C2 = 0.02 g/cm3C1 = 0.44 g/cm3

x2 x1 = 0.04 cm

Data:

1/28/2011

8

Chapter 5 - 15

Diffusing Species & Temperature example: carbon _ ironself-diffusion: D=3x10-21 m2/sinterdiffusion: D=2.4x10-12 m2/s

Factors That Influence Diffusion

Chapter 5 - 16

Diffusion and Temperature

Diffusion coefficient increases with increasing T.

D = Do exp

QdRT

= pre-exponential [m2/s]

= diffusion coefficient [m2/s]

= activation energy [J/mol or eV/atom]

= gas constant [8.314 J/mol-K]

= absolute temperature [K]

D

DoQdR

T

1/28/2011

9

Chapter 5 - 17

Diffusion and Temperature

Adapted from Fig. 5.7, Callister 7e. (Date for Fig. 5.7 taken from E.A. Brandes and G.B. Brook (Ed.) Smithells Metals Reference Book, 7th ed., Butterworth-Heinemann, Oxford, 1992.)

D has exponential dependence on T

Dinterstitial >> Dsubstitutional

C in -FeC in -Fe

Al in AlFe in -FeFe in -Fe

1000K/T

D (m2/s)

0.5 1.0 1.510-20

10-14

10-8T(C)15

00

1000

600

300

Chapter 5 - 18

Example: At 300C the diffusion coefficient and activation energy for Cu in Si are

D(300C) = 7.8 x 10-11 m2/sQd = 41.5 kJ/mol

What is the diffusion coefficient at 350C?

=

=

101

202

1lnln and

1lnln

TRQ

DDTR

QDD dd

==

121

212

11lnlnln

TTRQ

DD

DD d

transform data

D

Temp = T

ln D

1/T

1/28/2011

10

Chapter 5 - 19

Example (cont.)

= K 573

1K 623

1K-J/mol 314.8

J/mol 500,41exp /s)m 10 x 8.7( 2112D

=

1212

11exp

TTRQ

DD d

T1 = 273 + 300 = 573K

T2 = 273 + 350 = 623K

D2 = 15.7 x 10-11 m2/s

Chapter 5 - 20

Concept Check

Rank the magnitudes of the diffusion coefficients from greatest to least for the following systems:

N in Fe at 700oCCr in Fe at 700oCN in Fe at 900oCCr in Fe at 900oC

1/28/2011

11

Chapter 5 - 21

Non-steady State Diffusion

The concentration of diffucing species is a function of both time and position C = C(x,t)

In this case Ficks Second Law is used

2

2

xC

DtC

=

Ficks Second Law

Chapter 5 - 22

Non-steady State Diffusion

Adapted from Fig. 5.5, Callister 7e.

B.C. at t = 0, C = Co for 0 x

at t > 0, C = CS for x = 0 (const. surf. conc.)

C = Co for x =

Copper diffuses into a bar of aluminum.

pre-existing conc., Co of copper atoms

Surface conc., C of Cu atoms bars

Cs

1/28/2011

12

Chapter 5 - 23

Solution:

C(x,t) = Conc. at point x at time t

erf (z) = error function

erf(z) values are given in Table 5.1

CS

Co

C(x,t)

( )

=

Dtx

CCCt,xC

os

o

2 erf1

dye yz 2

0

2

=

Chapter 5 - 24

interpolation

1/28/2011

13

Chapter 5 - 25

Non-steady State Diffusion

Sample Problem: An FCC iron-carbon alloy initially containing 0.20 wt% C is carburized at an elevated temperature and in an atmosphere that gives a surface carbon concentration constant at 1.0 wt%. If after 49.5 h the concentration of carbon is 0.35 wt% at a position 4.0 mm below the surface, determine the temperature at which the treatment was carried out.

Solution: use Eqn. 5.5

=

Dtx

CCCtxC

os

o

2erf1

),(

Chapter 5 - 26

Solution (cont.):

t = 49.5 h x = 4 x 10-3 m Cx = 0.35 wt% Cs = 1.0 wt% Co = 0.20 wt%

=

Dtx

CCC)t,x(C

os

o

2erf1

)(erf12

erf120.00.120.035.0),(

zDtx

CCCtxC

os

o =

==

erf(z) = 0.8125

1/28/2011

14

Chapter 5 - 27

Solution (cont.):

We must now determine from Table 5.1 the value of z for which the error function is 0.8125. An interpolation is necessary as follows

z erf(z)0.90 0.7970z 0.81250.95 0.8209

7970.08209.07970.08125.0

90.095.090.0

=

z

z = 0.93

Now solve for D

Dtx

z2

=tz

xD

2

2

4=

/sm 10 x 6.2s 3600

h 1

h) 5.49()93.0()4(

m)10 x 4(

4211

2

23

2

2

==

=

tz

xD

Chapter 5 - 28

To solve for the temperature at which D has above value, we use a rearranged form of Equation (5.9a);

)lnln( DDRQ

To

d

=

from Table 5.2, for diffusion of C in FCC Fe